The increased demand for the development of alternative building materials has been encouraged by the growth of the building industry and the increased performance requirements together with the higher sustainability criteria applied in civil engineering. Alkali Activated Binders (AAB) represent an attractive alternative for the partial or complete substitution of Portland cement in the production of concrete and mortar. The potential benefit from the replacement of Portland cement by AAB is the reduction in carbon dioxide emissions. The production of 1 ton of Portland cement releases approximately 1 ton of carbon dioxide and requires about 100 kWh   . As opposed to this, the production of 1 ton of AAB creates only between 0.2 and 0.5 ton of carbon dioxide  -  . In comparison with composite cements or slag cements, the AAB is the better ecological solution as long as the amount of Portland cement is more than 50% by mass. Thereby, they offer more green benefits than commonly used
CEM II shows a minimum Portland cement portion of 65% by mass. Beyond this, AAB points up a high mechanical strength, a high temperature and fire resistance, an acid resistance and a low shrinkage  -  . Various scientific reports concerning the microstructure of different AAB are available   . Several current studies deal with the production of AAB and their durability properties   . The durability is a very controversial property of AAB. Some authors state it as the most important advantage over Portland cement, while others consider that as an unverified statement  -  . Similar to concrete, where a combination of mechanical and environmental loading can lead to the deterioration of mechanical properties, the durability of AAB is limited by material properties like water permeability, porosity, sorptivity, sulphate resistance, chloride ion penetration, carbonation, corrosion resistance, drying shrinkage and acid resistance   .
Actually, in comparison to Portland cement, the results of the latest research demonstrate better mechanical properties and durability under aggressive conditions for numerous reaction products made of AAB  -  . Furthermore, the investigations of Weil et al. show an outstanding durability for selective optimized AAB  . Malone already showed an enhanced frost resistance of AAB due to a comparatively high density and reduced porosity  . However, a noteworthy point is the formation of efflorescence products when AAB products are in contact with water or humidity  -  . The elution of the alkalis and their reaction with atmospheric carbon dioxide can lead to the formation of carbonates which appear as efflorescence on the surface    . An improvement of the durability can be implemented by a high amount of amorphous zeolite phases in the product realized by an adapted silicate modulus  .
Alkali activated binders are prepared by the alkaline activation of aluminosilicate materials such as fly ash, granulated slag or calcined clays   , and cured at ambient or slightly higher temperature   . The alkaline activation, which comprises the solving process, polymerization and crystallization, depends on many parameters, including chemical composition, physical properties (e.g. particle size distribution and specific surface area of the raw materials), composition of alkaline solution and curing temperature   . According to the law of mass action, the amount of amorphous phases formed by the reaction increases with increasing concentration of the alkaline solution  . Therefore, strength and durability increase, too  . For a further enhancement of mechanical properties of the AAB, short fibres can be integrated   .
This paper presents results of the development of an AAB-matrix with an emphasis on the measurement of the performance and durability of AAB-matrix.
2. Materials and Methods
2.1. Components for Alkali Activated Binders
In this study, the alkali activated binders were compared with an ordinary Portland cement concrete (OPCC). The compositions of the alkali activated binders are present in Table 1. For the reactive binders, the coal fly ash (bulk density: 2.42 g/cm³) “EFA-Füller” (class F) by the company Bauminerale GmbH and a granulated slag (bulk density: 2.85 g/cm³) by the company Holcim were used. The oxides compositions of the coal fly ashes and slag were determined by energy dispersive X-ray spectroscopy (EDX) and are shown in Table 2. The measured Blaine fineness of the coal fly ash and of the granulated slag was 7290 and 3740 cm²/g respectively. A quartz sand with a grain size of 0.1 to 1.0 mm was used as aggregate. The alkali resistant (AR) glass fibres, which lower the propensity to shrinkage cracking and can enhance first crack tensile strength in the concrete, were 12 mm long and had a length mass of 45 tex. The activator solutions consisted of a mixture of aqueous sodium silicate (SiO2/Na2O molar ratio: 2.1) and a solution of sodium hydroxide.
The sodium hydroxide solution was prepared by dissolving sodium hydroxide pellets (99% purity) in distilled water to a concentration of 2 - 10 mol/l and cooled to room temperature for 24 h. The water/binder ratio was 0.41.
Table 1. Composition of AAB and OPCC in wt%.
Table 2. Oxides compositions of coal fly ash and granulated slag in wt%.
2.2. Sample Preparation
The sodium hydroxide solution and the aqueous sodium silicate were stirred for 15 min by a magnetic stirrer. After that, the AAB specimens were manufactured by adding the activator solutions to the solid precursor (coal fly ash. granulated slag and aggregates). Then, all specimens were produced by mechanical mixing for 4 min. Subsequently, the AR-glass fibres were added to the fresh AAB and mixed together for 0.5 min. The detailed mixing proportion properties are shown in Table 3.
For the structural study of hardened AAB, the specimens were cast into corresponding molds and cured at a temperature of 20˚C and a relative humidity of 65% for 24 hours. Following this, the samples for the tests to be performed on the hardened concrete were stored dry, according to EN 12390-2.
2.3. Test Set-Up
The 3-point bending tensile strength was determined by means of the Toni Technik ToniNorm (load frame 20 kN) with three samples measuring 160 × 40 × 40 mm³ (length × width × height), based on EN12390-5 (Figure 1(a)). The compressive strength was determined by means of the Toni Technik ToniNorm (load frame 3000 kN) following EN 12390-3, with three cubes having an edge length of 150 mm (Figure 1(b)). The pre-load and the loading speed were 18 kN and 0.5 mm/min respectively.
Figure 1.Determination of 3-point bending tensile (a) and compressive strength (b).
Table 3. Composition of AAB and OPCC in wt%.
To quantify the durability of the AAB-matrix, the freeze-thaw test, the water permeability and the acid resistance were investigated. The freeze-thaw test was measured with the CIF-Test (Capillary suction, Internal damage and Freeze-thaw test) by the Schleibinger Freeze-Thaw-Tester with standard agent solution according to the recommendations of RILEM TC 176 IDC (Figure 2(a)). The acid resistance was determined by the mass loss after storage of three specimens (28 days old) in 37% hydrochloric acid for 7 days at a temperature of 21˚C (Figure 2(b)). The determination of the water permeability was carried out according to DIN EN 1062-3 (Figure 2(c)).
3. Results and Discussion
3.1. Properties of AAB
Table 4 reveals the fresh and hardened AAB characteristics at the age of 14 days. Using an air content tester, a gross geometric density of 2.39 g/cm³ and air content of 2.4 volume percent and were determined in the fresh AAB. The 3-point bending tensile and compressive strengths of the hardened AAB were 5.5 and 53.4 MPa respectively. The pH-value of the fresh AAB was 14, whereby the pH-value decreased to 10 due to the reactions in the hardened AAB. A dynamic elastic modulus of 36 GPa was determined by the ultrasonic examination. The total shrinkage deformation was 0.45 mm/m.
Furthermore to the reactivity and the solids content of the alkali activated binders, the amount and concentration of the alkaline activator have an influence on the solubility and reactivity of the AAB  . For this influence, the 3-point bending tensile
Figure 2.(a) CIF-Test; (b) Acid storage; (c) Water absorption.
Table 4. Basic properties of fresh and hardened AAB (NaOH: 5.5 mol/l).
strength (after seven days) is shown as a function of the NaOH concentration (1.2 to 10.0 mol/l) in Figure 3. Referring to Figure 3, an increase of the sodium hydroxide concentration leads to an increase of the 3-point bending tensile strength. The sodium hydroxide concentration of over 5.5 mol/l did not further increase the 3-point bending tensile strength, because the saturation point with respect to the solubility of the binder was reached, thus leading to a high level of degree of reaction. Sodium hydroxide concentrations over 5.5 mol/l did not result in an increasing of the 3-point bending tensile strength after seven days.
The thermogravimetry and the differential thermogravimetry of the AAB-matrix are illustrated in Figure 4. Regarding to Figure 4, it can be observed that the weight loss started at a temperature of 35˚C with maximum weight loss at 87˚C. This weight loss can be attributed to the removal of free and unbound absorbed water molecules. The further mass loss up to a temperature of about 300˚C corresponded to the physically bound water in the porous matrix and the zeolite-water from the nanocrystalline zeolite structures   . The mass loss up to a temperature of around 520˚C resulted from the decomposition of the chemically bound water from the calcium silicate and the calcium aluminate phases. The cumulated weight loss was of 10.5% at a temperature of 900˚C.
3.3. Durability of AAB Matrix
The results of the durability of the alkali activated binder were investigated and the comparison with the ordinary Portland cement concrete is shown in Table 5. The results comprise the freeze-thaw test, the water permeability and the acid resistance. The AAB-matrix had a water absorption coefficient (wt) of 0.095 kg/m²∙h0.5 and reached the class 3 (low water absorption) according to DIN EN 1062-3 (Table 5). As opposed to this, the OPCC had a water absorption coefficient of 1.301 kg/m²∙h0.5 and reached the class 1 (high water absorption).
Table 5. Results of the durability of AAB and OPCC.
Figure 3. 3-point bending tensile strength as a function of the NaOH concentration.
Figure 4. Thermogravimetry and the differential thermogravimetry of the AAB.
In addition, the AAB-matrix exhibited a high frost resistance, which was verified through a successful CIF test with a relative dynamic modulus of elasticity of 93 percent (Ru, 28) and an average scaling of 30 g/m² (m28) after 28 freeze-thaw cycles (Table 5 and Figure 5).
After seven days storage in 37% hydrochloric acid, the AAB-matrix had a mass loss of 15.9% (see Table 5 and Figure 6). In comparison, the mass loss of the OPCC was significantly higher with 75.9%. The high acid resistance of the AAB-matrix is mainly due to the portlandite-free phases.
Figure 5. Test surface before (a) and after (b) the CIF-Test.
Figure 6. AAB and OPCC samples before (left) and after the acid attack (right).
In this study herein, the development of an AAB-matrix and the performance and durability of different fibres in the AAB-matrix were investigated through various experimental work. Based on the results of this study, the following key points are drawn:
- The adapted molarity of the sodium hydroxide solution was 5.5 mol/l. Sodium hydroxide concentrations over 5.5 mol/l did not result in an increasing of the 3-point bending tensile strength after seven days,
- The AAB achieved a compressive and a 3-point bending tensile strength of 53.4 and 5.5 MPa respectively after one day at ambient temperatures,
- The acid resistance of the AAB was 500% higher than the ordinary Portland cement concrete, which could be attributed mainly to the free portlandite phases.
This work was supported by the German Federation of Industrial Research Associations (AiF). The authors would like to acknowledge with gratitude the foundation’s financial support.
http://dx.doi.org/10.1021/es202190r  IEA (2009) Cement Technology Roadmap 2009. Carbon Emissions Reductions up to 2050.  McLellan, B.C., Williams, R.P., Lay, J., van Riessen, A. and Corder, G.D. (2011) Costs and Carbon Emissions for Geopolymer Pastes in Comparison to Ordinary Portland Cement. Journal of Cleaner Production, 19, 1080-1090.
http://dx.doi.org/10.1016/j.jclepro.2011.02.010  Davidovits, J. (1993) Geopolymer Cements to Minimise Carbon Dioxide Greenhouse Warming. Ceramic Transactions, 37, 165-182.  Komnitas, K. and Zaharaki, D. (2007) Geopolymerisation: A Review and Prospects for the Minerals Industry. Minerals Engineering, 20, 1261-1277.
http://dx.doi.org/10.1016/j.mineng.2007.07.011  Shi, C., Jimenez, A. and Palomo, A. (2011) New Cements for the 21st Century: The Pursuit of an Alternative to Portland Cement. Cement and Concrete Research, 41, 750-763.
http://dx.doi.org/10.1016/j.cemconres.2011.03.016  Bernal, S.A., et al. (2014) MgO Content of Slag Controls Phase Evolution and Structural Changes Induced by Accelerated Carbonation in Alkali-Activated Binders. Cement and Concrete Research, 57, 33-43.
http://dx.doi.org/10.1016/j.cemconres.2013.12.003  Funke, H. and Gelbrich, S. (2015) Alkalisch aktivierte Bindemittel zur Generierung von faserverst?rkten Vergussmassen. 19. Ibausil, Weimar, 16-18 September 2015, Band 1, 859- 866.  Murmu, M. and Singh, A. (2014) Hydration Products, Morphology and Microstructure of Activated Slag Cement. International Journal of Concrete Structures and Material, 8, 61-68.  Kar, A., Ray, I., Halabe, U.B., Unnikrishnan, A. and Dawson-Andoh, B. (2014) Characterizations and Quantitative Estimation of Alkali-Activated Binder Paste from Microstructures. International Journal of Concrete Structures and Materials, 8, 213-228.
http://dx.doi.org/10.1007/s40069-014-0069-0  Provis, J.L. (2014) Geopolymers and Other Alkali Activated Materials: Why, How, and What? Materials and Structures, 47, 11-25.
http://dx.doi.org/10.1617/s11527-013-0211-5  Vance, K., Aguayo, M., Dakhane, A., Ravikumar, D., Jain, J. and Neithalath, N. (2014) Microstructural, Mechanical, and Durability Related Similarities in Concretes Based on OPC and Alkali-Activated Slag Binders. International Journal of Concrete Structures and Materials, 8, 289-299.
http://dx.doi.org/10.1007/s40069-014-0082-3  Sakulich, A.R. (2011) Reinforced Geopolymer Composites for Enhanced Material Greenness and Durability. Sustainable Cities and Society, 1, 195-210.
http://dx.doi.org/10.1016/j.scs.2011.07.009  Pacheco-Torgal, F., Castro-Gomes, J. and Jalali, S. (2008) Alkali-Activated Binders: A Review Part 1. Historical Background, Terminology, Reaction Mechanisms and Hydration Products. Construction and Building Materials, 22, 1305-1314. http://dx.doi.org/10.1016/j.conbuildmat.2007.10.015  Hossain, M., Karim, M.R., Hossain, M.K., Islam, M.N. and Zain, M.F.M. (2015) Durability of Mortar and Concrete Containing Alkali-Activated Binder with Pozzolans: A Review. Construction and Building Materials, 93, 95-109.
http://dx.doi.org/10.1016/j.conbuildmat.2015.05.094  Bondar, D., Lynsdale, C.J., Milestone, N.B. and Hassani, N. (2015) Sulfate Resistance of Alkali Activated Pozzolans. International Journal of Concrete Structures and Materials, 9, 145-158.
http://dx.doi.org/10.1007/s40069-014-0093-0  Pacheco-Torgal, F. and Jalali, S. (2011) Resistance to Acid Attack, Abrasion and Leaching Behavior of Alkali-Activated Mine Waste Binders. Materials and Structures, 44, 487-498.
http://dx.doi.org/10.1617/s11527-010-9643-3  Deb, P., Nath, P. and Sarker, P. (2014) The Effects of Ground Granulated Blast-Furnace Slag Blending with Fly Ash and Activator Content on the Workability and Strength Properties of Geopolymer Concrete Cured at Ambient Temperature. Materials and Design, 62, 32- 39.
http://dx.doi.org/10.1016/j.matdes.2014.05.001  Ismai, I., Bernal, S.A., Provis, J.L., Hamdan, S. and van Deventer, J.S.J. (2011) Microstructural Changes in Alkali Activated Fly Ash/Slag Geopolymers with Sulfate Exposure. Materials and Structures, 46, 361-373.
http://dx.doi.org/10.1617/s11527-012-9906-2  Ismail, I., et al. (2013) Influence of Fly Ash on the Water and Chloride Permeability of Alkaliactivated Slag Mortars and Concretes. Construction and Building Materials, 48, 1187- 1201.
http://dx.doi.org/10.1016/j.conbuildmat.2013.07.106  Yang, T., Yao, X. and Zhang, Z. (2014) Quantification of Chloride Diffusion in Fly Ash- Slag-Based Geopolymers by X-Ray Fluorescence (XRF). Construction and Building Materials, 69, 109-115.
http://dx.doi.org/10.1016/j.conbuildmat.2014.07.031  Weil, M., Dombrowski-Daube, K. and Buchwald, A. (2011) Geopolymer Binders—Part 3: Ecological and Economic Analyses of Geopolymer Concrete Mixes for External Structural Elements. ZKG International, 64, 76-87.  Malone, P., Randall, C. and Kirkpatrick, T. (1985) Potential Applications of Alkali-Acti- vated Alumino-Silicate Binders in Military Operations. US Army Corps of Engineers, Miscellaneous Paper.  Kani, E., Allahverdi, A. and Provis, J. (2011) Efflorescence Control in Geopolymer Binders Based on Natural Pozzolan. Cement and Concrete Composites, 34, 25-33.
http://dx.doi.org/10.1016/j.cemconcomp.2011.07.007  Zhang, Z., Provis, J.L., Reid, A. and Wang, H. (2014) Fly Ash-Based Geopolymers: The Relationship between Composition, Pore Structure and Efflorescence. Cement and Concrete Research, 64, 30-41.
http://dx.doi.org/10.1016/j.cemconres.2014.06.004  Yao, X., Yang, T. and Zhang, Z. (2015) Compressive Strength Development and Shrinkage of Alkaliactivated Fly Ash-Slag Blends Associated with Efflorescence. Material and Structures, 49, 2907-2918.
http://dx.doi.org/10.1617/s11527-015-0694-3  Fiala, C., Mukarovsky, J. and Kynclova, M. (2008) Material Effective Structures—The Way towards Sustainable Buildings. Proceedings of the Conference on Sustainable Building SB08 Melbourne, Melbourne, 21-25 September 2008, 196-203.  Pacheco-Torgal, F., Abdollahnejad, Z., Camoes, A.F., Jamshidic, M. and Ding, Y. (2012) Durability of Alkali-Activated Binders: A Clear Advantage over Portland Cement or an Unproven Issue? Construction and Building Materials, 30, 400-405.
http://dx.doi.org/10.1016/j.conbuildmat.2011.12.017  Damtoft, J., Lukasik, J., Herfort, D., Sorrentino, D. and Gartner, E.M. (2008) Sustainable Development and Climate Change Initiatives. Cement and Concrete Research, 38, 115-127.
http://dx.doi.org/10.1016/j.cemconres.2007.09.008  Davidovits, J. (1991) Geopolymers: Inorganic Polymeric New Materials. Journal of Thermal Analysis, 37, 1633-1656.
http://dx.doi.org/10.1007/BF01912193  Cheng, T.W. (2010) Development and Application of Geopolymer Technology: A Review. Mining and Metallurgy, 54, 141-157.  Schneider, M., Romer, M., Tschudin, M. and Bolio, H. (2011) Sustainable Cement Production—Present and Future. Cement and Concrete Research, 41, 642-650.
http://dx.doi.org/10.1016/j.cemconres.2011.03.019  Duxson, P., Provis, J.L., Lukey, G.C. and van Deventer, J.S.J. (2007) The Role of Inorganic polymer Technology in the Development of Green Concrete. Cement Concrete Research, 37, 1590-1597.
http://dx.doi.org/10.1016/j.cemconres.2007.08.018  Duxson, P., Lukey, G. and van Deventer, J. (2007) The Thermal Evolution of Metakaolin Geopolymers: Part 2—Phase Stability and Structural Development. Journal of Non-Crys- talline Solids, 352, 5541-5555.
http://dx.doi.org/10.1016/j.jnoncrysol.2006.09.019  Wang, H., Li, H. and Yan, F. (2005) Synthesis and Mechanical Properties of Metakaolinite-Based Geopolymer. Colloids and Surfaces A: Physiochemical and Engineering Aspects, 268, 1-6.
http://dx.doi.org/10.1016/j.colsurfa.2005.01.016  Li, W. and Xu, J. (2009) Mechanical Properties of Basalt Fibre Reinforced Geopolymeric Concrete under Impact Loading. Materials Science Engineering, 505, 178-186.
http://dx.doi.org/10.1016/j.msea.2008.11.063  Funke, H., Gelbrich, S., Ehrlich, A. and Kroll, L. (2014) Rheological and Mechanical Development of a Fiber-Reinforced Concrete for an Application in Civil Engineering. SOJ Materials Science & Engineering, 2, 1-4.
http://dx.doi.org/10.15226/sojmse.2014.00111  Buchwald, A. (2012) Der Einfluss des Kalziums auf die Kondensation von (Alumo-)Silika- ten in alkali-aktivierten Binder. Habilitation Thesis, Gemeinsamer Bibliotheksverbund, Erfurt.  Provis, J., Lukey, G. and Deventer, J. (2005) Do Geopolymers Actually Contain Nanocrystalline Zeolites? A Reexamination of Existing Results. Chemistry of Materials, 17, 3075- 3085.
http://dx.doi.org/10.1021/cm050230i  Bernal, S. (2011) Mechanical and Thermal Characterization of Geopolymers Based on Silicate Activated Metakaolin/Slag Blends. Journal Material Science, 46, 5477-5486.